HAL Id: jpa00211089
https://hal.archivesouvertes.fr/jpa00211089
Submitted on 1 Jan 1989
HAL is a multidisciplinary open access archive for the deposit and dissemination of sci entific research documents, whether they are pub lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
On the calculation of the interaction energy of defects in metals
E. Daniel, C. Koenig
To cite this version:
E. Daniel, C. Koenig. On the calculation of the interaction energy of defects in metals. Journal de
Physique, 1989, 50 (18), pp.26372646. �10.1051/jphys:0198900500180263700�. �jpa00211089�
2637
On the calculation of the interaction _{energy } of defects in metals
E. Daniel and C. Koenig
Université Louis Pasteur  I.P.C.M.S., ^{4 } ^{rue } Blaise Pascal, 67070 Strasbourg Cedex, ^{France}
(Reçu ^{le 6 } ^{mars } ^{1989, } accepté le Il avril 1989)
Résumé.
^{2014 }On montre qu’on peut calculer de façon ^{cohérente } l’énergie d’interaction de deux défauts dans un métal à partir ^{de } potentiels effectifs obtenus en aplatissant les oscillations de Friedel de la densité de charge électronique audelà d’une distance définie de chaque ^{défaut.}
Abstract.
^{2014 }It is shown that the interaction energy of ^{two } defects in a metal can be computed consistently from oneelectron effective potentials ^{obtained } by flattening ^{out } the Friedel oscillations of the electron charge density beyond ^{a } definite distance from each defect.
J. Phys. ^{France } ^{50 } (1989) ^{26372646 } ^{15 } ^{SEPTEMBRE } ^{1989,}
Classification
Physics ^{Abstracts}
71.55DP
1. Introduction.
The Friedel theory ^{of the } screening ^{of } point defects in a metal [1] constitutes for metallic
alloys ^{an } achievement comparable ^{to } ^{that } accomplished by Sommerfeld [2] for pure metals with the free electron gas obeying FermiDirac statistics. In both cases quantum ^{effects } ^{are} essential.
The celebrated Friedel sumrule :
relates the screening charge ^{Z } ^{to } ^{the } phase ^{shifts } ru produced by the defect potential ^{in the} spherical partial ^{waves } of orbital momentum f at the Fermi level _{EF } of the conduction electrons of the metal, ^{when } represented by ^{a } free electron gas. This rule shows clearly ^{how}
the electronic screening charge ^{of } ^{an } impurity ^{atom } ^{B } dissolved in an otherwise pure metal A builds up in order to restore locally ^{more or } ^{less } of its neutral atom character to the B element. This charge ^{extends } roughly ^{to } the atomic sphere ^{of B } ^{but, } simultaneously, ^{the} phase ^{shifts } produced in the different spherical components of the wavefunctions result in ^{an}
oscillating ^{variation } of the electron density p (r ) in the metal A, ^{with } ^{an } asymptotic ^{behaviour}
at large distance r from B :
where kF ^{is } the Fermi radius of the electron gas and q ^{some } average phase shift. This is
basically ^{a } quantum effect related to the discontinuity ^{of } occupation of the electron states at
Article published online by EDP Sciences and available at http://dx.doi.org/10.1051/jphys:0198900500180263700
the Fermi level. It is then obvious that these Friedel oscillations of the electronic charge density ^{must } give ^{rise } ^{to } long range interactions between defects in a metal [3]. ^{In } ^{the } ^{case } ^{of} magnetic impurities, they ^{lead } ^{to } spin glasses [4].
For going from the free electron Sommerfeld theory ^{to } ^{a } quantitative ^{treatment } of real pure
metals, ^{it } ^{was } necessary ^{to } introduce the crystalline periodic potential into the band structure calculations and to take the Coulomb electronelectron interactions into account. Efficient numerical techniques have been devised for that and are extensively used with modern
computing facilities. Some of the methods used in selfconsistent band structure calculations
can be rather naturally ^{extended } ^{to } the electronic structure of defects or impurities ^{in dilute} alloys ^{or } ^{metallic } compounds ; they integrate then the energy spectrum of the Bloch states of the electron valence bands which are scattered by the defect. This is the case, for instance, ^{for}
the Green function method [5] ^{or } the method of linearized « muffintin » orbitals in the atomic sphere approximation (LMTOASA) [6]. ^{Numerous } applications of these methods have been made during ^{the last } decade, generally ^{in } good quantitative agreement ^{with} experimental ^{data.}
At first sight, ^{a } major difficulty arises when one wishes to perform ^{a } selfconsistent calculation of the interaction energy of ^{two } defects in a metal. Each of them creates long
range electron charge density oscillations, ^{so } that, strictly speaking, ^{no } ^{atom } is neutral any
more. The charges ^{of } ^{a } given sign integrated ^{in } ^{a } spherical shell of radius ^{r } decrease only ^{as} r1 and the successive shells interfere very far from each scattering ^{center. } This makes it
illusory ^{to } attempt ^{a } fully selfconsistent calculation. This state of affairs is corroborated by
the following remark made by ^{Stefanou } ^{while } computing ^{the } charge ^{and } spin densities around
a vanadium impurity dissolved in nickelmetal [7]. By increasing progressively the number of atomic shells included in a cluster treated selfconsistently around the vanadium atom, ^{he} found that the electronic density stabilized itself rather rapidly inside the cluster while the
oscillating charge density ^{outside } changed completely ^{at } ^{each } step.
Nevertheless, ^{it } ^{seems } possible ^{to } compute significant values for the interaction energy of defects even if the precise charge density ^{at } large ^{distances } ^{cannot } be calculated. Most of the present calculations of the electronic structure of metallic materials are based on the variational principle ^{of } Hohenberg ^{and Kohn } according ^{to } the Kohn and Sham for mulation [8]. Exchange and electron correlation effects are usually taken into account in the local density approximation through ^{the } HedinLundqvist interpolation ^{formula } [9]. ^{Accord} ing ^{to } the variational principle, given the electrostatic potential ^{v } ^{of the } nuclei, ^{the } ground
state total energy of the electronnuclei system ^{is } equal ^{to } the minimum value of ^{some} functional E, [p ] of the electronic density p (r), this value being obtained for the true self consistent electronic density. ^{A } slightly ^{different } density p’, ^{if close } enough ^{to } ^{p, } ^{will } ^{not} change the total energy ^{to } first order and so can be used in a numerical calculation. This property has often been used in more or less equivalent forms for different applications, ^{for}
instance the total energy and compressibility ^{of } homogeneous crystals [10] ; it underlies the Natta and Toulouse proof [11] ^{made } ^{on an } approximate tightbinding model that the interaction energy of ^{two } point defects in a metal must decrease according ^{to } ^{the} r 3 law at large distances ; ^{this work } ^{was } exploited ^{later } ^{on } ^{in } tightbinding models of dilute
alloys involving transition metal impurities [12].
The purpose of the present article is to derive ^{a } precise prescription ^{for the } ^{abinitio}
calculation of the interaction energy of ^{two } defects in a metal. For simplicity, the derivation will be formulated for the case of two « point ^{defects } ^{» } although the method is quite general
and could be extended in an obvious way ^{to } many other ^{cases } such as, for insance, ^{the}
interaction energy between ^{an } impurity ^{atom } ^{and } ^{a } ^{surface. } Exchange and correlation effects
will be considered only in the local density approximation.
2639
2. Total energy with ^{an } approximate ^{électron } density.
Following Kohn and Sham theory, ^{the } ground ^{state } total energy of ^{a } system of electrons with
density p (r) in the electrostatic potential v (r) of fixed nuclei is the minimum value of the
density functional :
where T[p ] ] is the kinetic energy of ^{a } noninteracting electron gas with the ^{same } density
p (r) ^{in } ^{an } appropriate ^{effective } potential veff (r) ^{which has } ^{to } ^{be found } selfconsistently, ^{and} E,,c [p ] defines the exchange and correlation energy. In the local density approximation, ^{one}
takes :
êxC (p) being ^{the } exchange ^{and } correlation energy of ^{a } homogeneous electron gas with constant density ^{p. } ^{For } ^{an } infinitesimal variation &p of the electron charge density ^{such } ^{as } ^{to} keep the total number of electrons constant, ^{one } gets :
where :
defines the ^{« } exchange ^{and } correlation potential ^{». } ^{For } ^{the } ^{same } ^{variation } 8p, ^{the } change ^{in}
energy of the associated noninteracting ^{electron } system ^{is :}
The condition of minimum :
determines the effective potential :
This potential ^{must } ^{be } computed selfconsistently through ^{an } ^{iterative } procedure ^{from the}
oneelectron Schrôdinger equation :
Let n (e ) ^{be the } density ^{of } ^{states } per unit of energy in this noninteracting system ; ^{then :}
Suppose ^{now } ^{that } ^{p } (r) ^{is } slightly ^{modified } by ^{a } ^{small } change 8 p ^{such } ^{as } ^{to } keep ^{the total}
number of electrons constant ; this defines an approximate density :
with:
The effective potential corresponding ^{to } ^{p ’ } ^{is :}
From the variational principle, the total energy does ^{not } change ^{to } first order in
Likewise, ^{the } density ^{variation } 8 p ^{in the } noninteracting system being made with the effective
potential kept ^{constant :}
so that :
and :
From the explicit ^{form of } Veff, ^{one } gets :
with :
^{O }^{O}Let : with : Im ^{E = } + 0, ^{be the } ^{Green } operator ^{for the } ^{non}
interacting system ^{with } Veff ^{and let } G’(E) ^{be } ^{the } ^{Green } operator corresponding ^{to} v’ ; they ^{are } ^{related } through ^{the } Dyson equation :
to first order in ou.
2641
To this approximation, the difference of the densities of states per unit of energy is :
Let : be the total number of electrons up ^{to } energy e ^{and let} N’ be the corresponding quantity for v’ ; ^{to } first order in 5 v :
and :
so that :
after integration by parts ^{on } ^{E.}
Finally :
3. Interaction _{energy } of two ^{« } points ^{defects ».}
As far as the rearrangement ^{of } charge ^{due } ^{to } the interaction of the defects is small, ^{it } ^{seems}
reasonable to take as approximate density p’ ^{the } density ^{obtained } by rigid superposition ^{of}
the screening charges associated with each of the defects when alone in the metal. These
screening charges ^{must } ^{be } computed selfconsistently beforehand for the single defects. This is far less difficult than the direct selfconsistent calculation of the electronic structure of the
pair of defects.
Let p (r ) be the electron charge density in the pure metal, p 1 (r ) that of the metal containing
the first defect alone at Rl, P 2 (r) that of the metal with the second defect alone at
R2 ^{and } finally, ^{let } Pl, 2 (r) be the unknown selfconsistent electron charge density ^{when both}
defects are present in the metal. Let Zl ^{be the } screening charge associated with the first
defect, Z2 ^{that } corresponding ^{to } the second defect. With similar indices for the total numbers of electrons, it is clear that :
and
because one or two localized defects in an arbitrary large volume of metal ^{cannot } change ^{the}
Fermi level.
The interaction energy of the defects is ^{now } defined as the difference in total energies :
with :
As mentioned earlier in the introduction, ^{it } ^{is } illusory ^{to } attempt ^{to } compute ^{self} consistently p 1 (r) ^{and } p 2 (r ) beyond ^{a } few atomic layers around the defects. Fortunately, by
virtue of the variational principle, ^{this is } ^{not } necessary. The screening charge associated with a
defect being mostly ^{localized } in its atomic sphere ^{or } ^{so, } ^{the } variation of the charge integrated
from the defect outwards oscillates around the value corresponding ^{to } ^{the } ^{exact } screening.
There is an infinite number of closed surfaces, ^{centered } ^{on } ^{the } defect, each of them enclosing
the exact screening charge while the oscillations of the density become smaller and smaller outside. It is then possible, by flattening the oscillations on the outside of such a surface, ^{to} obtain an approximate density of electron charge p Í valid for the calculation of the energy of the defect located at R, ^{and, } similarly, ^{a } good approximate density p2 for the second defect.
As far as second order corrections are negligible, ^{the } interaction energy ^{can } be written in terms of the approximate densities :
with :
When taking ^{into } ^{account } ^{the } ^{Coulomb } repulsion between the nuclei, this leads to the
following expression ^{for the } interaction energy :
with the exchange correlation correction :
f2l 1 and f2 2 being the volumes kept around each defect and in which, respectively, p 1 ^{or } p’ 2 differ from p.
Usually, the electronic charge density changes produced by ^{a } ^{defect } ^{on } the outside of its
own atomic cell are rather weak, typically of the order of one tenth or even one hundredth of
a unit of charge per atomic cell. Under these conditions, ^{it is } permissible ^{to } linearize the
corresponding change ^{in } exchange ^{and } correlation energy. The exchange and correlation
correction disappears ^{then } ^{to } ^{first } ^{order, } ^{except } in the atomic cells _{cri } and _{(T2 } of the defects
and one is left with :
2643
where 8NÍxC«(T2) is the contribution to N i of the change ^{in the } exchangecorrelation potential
in (T2 with respect ^{to } the pure metal, and similar meaning for the other terms. So, thé exchangecorrelation correction 8Exc completely drops ^{out } provided ^{that the } exchange ^{and}
correlation modifications of the potentials ^{are } ^{not } made. This means that Ni i ^{and} N2 ^{should be } computed with the full potential, exchange and correlation included, ^{in the}
atomic cells of the defects, ^{but with } only the Hartreelike Coulomb corrections with respect ^{to} the pure metal in il 1  (T 1 and il 2  (T 2 respectively. ^{From the } linearity of the relation between electric charge and Coulomb potential, ^{the } perturbative potential Vi’ 2 ^{of } ^{the } pair ^{of}
defects in which N r, 2 ^{must } ^{be } ^{computed } ^{is just } ^{the } ^{sum :}
of the perturbative potentials ^{in } ^{which } Ni ^{and } N2 ^{are } calculated. These potentials,
constructed as explained above, ^{are } ^{not } selfconsistent and do not attract the exact screening charge, ^{but } they ^{must } give ^{the } ^{correct } interaction energy according ^{to } the final formula :
in which the last integral represents the Coulomb interaction of the two screening ^{electron}
clouds which is counted twice in the oneelectron part.
The oneelectron integral ^{can } be written in terms of the Green operator G for the pure
metal, ^{and those } corresponding respectively ^{to } V i , V2 ^{and } VI’ 2. ^{From the } Dyson equation :
and similar relations with V2 ^{and } V 1", ^{2, one } ^{gets } ^{for } ^{two } spin directions :
so that :
the determinant can be factorized in a way appropriate ^{for } numerical calculation.
Let us take for illustration ^{the } simple ^{model of } ^{a } single tightbinding ^{band with } ^{two}
perfectly ^{screened } impurity ^{atoms, } ^{one } ^{at } ^{the } origin : RI
^{= }0 and the second at R2
^{= }^{R :}
all other matrix elements being ^{zero. } ^{In this } model, the corrective term disappears ^{because}
the localized screening charges neutralize exactly the nuclear terms and one is left with the oneelectron contribution :
In lowest order in perturbation, ^{this } gives :
In the limit of large R, ^{with } ^{a } free electron approximation ^{for the } dispersion ^{law } in the band :
k being the electron wave vector and va, the atomic volume, one recovers the asymptotic
behaviour of the linear response theory :
with nat ( £F) being ^{the } density of electron states per ^{atom } and unit of energy.
4. Discussion.
In the ideal case where each defect is perfectly screened in its own atomic cell, the Coulomb interaction of the screening ^{clouds } compensates the nuclear repulsive ^{term } ^{in } the atomic
sphere approximation ^{so } that the corrective term disappears totally, except ^{for } high ^{order} multipolar ^{terms } ^{which } ^{must } be very small in compact crystalline structures. Eint ^{is then } given by ^{the } ^{one } electron contribution alone. It is clear in that case that the interaction energy results from the multiple scattering of the conduction electrons by ^{the } pair ^{of } screened,
therefore neutral, defects and is not given by ^{the } product of the ionic charge ^{of } ^{one } ^{of them in}
the Coulomb potential ^{created } by ^{the other } ^{one on } ^{its } site. A similar remark was already
made by ^{Caroli } [13] ^{for the } coupling between the localized magnetic ^{moments } associated with two virtual bound states. One should not forget that the screened potential ^{of } ^{an } impurity
atom is not weak in its own cell ; it may give ^{rise } ^{to } resonances or even substract bound states out of the conduction band ; only ^{on } the outside of this cell can it be considered as a small
perturbation.
In many real cases, the defect is underscreened in its own atomic cell and the screening charge ^{involves } ^{its } neighbouring ^{atoms. } ^{This } ^{is } ^{so, } ^{for } instance, for vacancies in metals or
metallic compounds ^{such } ^{as } ^{FeAl } [14]. The conduction electrons tunnel easily through ^{the}
vacancies which in some cases can retain up ^{to } ^{one } electron charge ^{which has } ^{to } ^{be } ^{borrowed}
from the neighbouring ^{atoms. } ^{In such } ^{cases, } ^{the } ^{volume fi } of the cluster to be treated self
consistently ^{must } ^{include } ^{at } ^{least the } ^{first } ^{nearest } neighbour shell. When the defects are close
enough ^{so } that their screening charges overlap, the corrective term becomes important. ^{It is}
2645
then essential that each individual cluster be neutral in order to avoid errors much larger ^{than}
the correction itself.
In order to illustrate the influence of the overlap ^{of the } screening charges ^{when } ^{no } ^{cutoff is}
made on the oscillations, ^{we } have calculated the Coulomb interaction energy correction
,6E(R) ^{for } ^{two } ^{defects } ^{at } ^{a } distance R apart, each defect being ^{simulated } by ^{a } ^{hardcore} pseudopotential ^{of radius } ^{a } repelling exactly ^{one } electron in the ^{« } s » partial ^{waves } ^{of } ^{a } ^{free}
electron gas (Fig. 1). ^{From the } screening ^{condition } for the individual defects, ^{one } ^{has :}
2 kF a
^{= }^{7T, } ^{so } ^{that } kF
^{= }^{1 } ^{a.u. } ^{would } give a = ’r ^{a.u. } ^{while the } atomic radius would be : 2
rs = 1.92 ^{a.u. } On the same picture ^{are } plotted ^{the } potential energy V (R ) ^{for } ^{an } ^{electron } ^{at}
R
distance R from a single ^{screened } ^{defect } ^{and the } screening charge : Q (R )
^{= }^{4 } ^{7T }
p ^{0} ^{(r) } ^{r2 dr}
inside a sphere of radius R. One sees that SE(R) ^{becomes } rapidly much smaller than
V (R ) but in order to get ^{a } ^{correct } result when the two defects are but a few atomic distances apart, it is necessary ^{to } integrate up ^{to } about one hundred times the radius in which the right screening charge Q
^{=  }^{1 } is obtained for the first time. Moreover, ^{if } ^{one } puts ^{a } ^{cutoff } ^{on } ^{the} radius of the sphere in which the screening charge Q (r) is taken into account, ^{then the}
Fig. ^{1. }
^{ }Coulomb correction to the interaction energy of ^{two } defects in a free electron gas, ^{versus } the distance separating these defects : a : radius of the hardcore pseudopotentials ; 6(7?) : screening charge ^{inside } ^{a } sphere ^{of radius } ^{R for } ^{one } ^{defect } (  ) ; V (R ) : potential energy of ^{one } electron at a
distance R of one screened defect () ; SE(R) : total interaction energy correction for ^{two } screened
defects separated by ^{a } ^{distance } ^{R } ( ) .
numerical calculation shows that the error made on 8 E (R ) may be ^{more } than one order of
magnitude larger than the value 8 E (R ) ^{to } ^{be } computed ^{if } G(r) ^{is } ^{not } equal ^{to}
